Innovative Systems Design and Engineering www.iiste.orgISSN 2222-1727 (Paper) ISSN 2222-2871 (Online) Characterization study on the variation of weight percentage of Alumina Aluminum in-situ Particulate reinforced composite material K.S.Raghuram (Corresponding Author) Associate Professor, Department of Mechanical Engineering, Sri Chaitanya Engineering College, Visakhapatnam, A.P. Cell:9550013119 email:firstname.lastname@example.org Dr. N.V.S.Raju Associate Professor, Department of Mechanical Engineering, JNTU College of Engineering, Nachupalli, Kondagattu, Karimnagar, A.P. Cell: 8008102125 email: email@example.comAbstractIN-SITU Al2O3 SiC C having 20 wt%, 25 wt%, 30 wt% and 35wt% of powdered particulate were fabricated byliquid metallurgy (stir cast) method. The composite specimens were machined as per test standards. The specimenswere tested to know the common casting defects using image analyzer. Some of the mechanical properties havebeen evaluated and compared with Al6061 alloy. Significant improvement in uniform distribution of particulates isnoticeable as the wt % of the flake particles increases. The microstructures of the composites were studied to knowthe dispersion of the powdered particles in the matrix. It has been observed that addition of flake particlessignificantly improves particulate distribution.Keywords: flake particles, Al - Al2O3SiC C matrix composite, image analyzer, particulate distribution properties.INTRODUCTIONMetal Matrix Composites are being increasingly used in aerospace and automobile industriesowing to theirenhanced properties such as elastic modulus, hardness, tensile strength at roomand elevated temperatures, wearresistance combined with significant weight savings over unreinforced alloys [1-4]. Aluminum is the commonlyused metallic matrix. These alloys are preferred matrix materials for the production of MMCs. The reinforcementsbeing used are fibers, whiskers and particulates . The advantages of the particulate-reinforced composites overothers are their formability with cost advantage .The various MMCs & their applications are mentioned in Table 1 as shown below.The strengthening of particulate MMC may be due to different mechanisms. Orowan strengthening Grain and sub-structure strengthening Quench strengthening Work hardening.Hence the particulate having Al2O3 SiC C in powder form with 30 μm is selected for reinforcement in whiskerform. Low strength alloys (eg. Pure Aluminum) are greatly strengthened by ceramic phased e.g. SiC particulates.For high strength alloys (e.g. 2xxx or 7xxx alloys), there is an effect of the reinforcement on the age hardening. Insome alloys (e.g. 7xxx series), it is difficult to reach the same strength in the composite as in the monolithic alloy,for 2xxx and 7xxx based composites, the strength of the composite may be 100 MPa higher than the starting matrixalloy.
Innovative Systems Design and Engineering www.iiste.orgISSN 2222-1727 (Paper) ISSN 2222-2871 (Online)Here the technique used is grain and sub-structure strengthening. Further, they are inherent with heat and wearresistant properties [7, 8]. For MMCs SiC, Al2O3and C are widely used particulate reinforcements. The ceramicparticulate reinforced composites exhibit improved abrasion resistance . They find applications as cylinderblocks,pistons, piston insert rings, brake disks and calipers . The strength of these composites is proportional tothe percentage volume and fineness of the reinforced particles . These ceramic particulate reinforced Al-alloycomposites led to a new generation tailorable engineering materials with improved specific properties [12, 13]. Thestructure and the properties of thesecomposites are controlled by the type and size of the reinforcement and also thenature of bonding [14-16]. From the contributions of several researchers, some of the techniques for thedevelopment of these composites are stir casting , powder metallurgy , spray atomizationand co-deposition, plasma spraying  and squeeze-casting . The above processes are most important of which, liquidmetallurgy technique has been explored much in these days and hence the present paper summarizes the studiesconducted by several investigators under sections characterization and particulate distribution.Density is the physical property that reflects the characteristics of composites. In a composite, the proportions of thematrix and reinforcement are expressed either as the weight fraction (w), which is relevant to fabrication, or thevolume fraction (v), which is commonly used in property calculations. By relating weight and volume fractions viadensity (ρ), the following expression is obtained (m stands for matrix, c for the composite and r for reinforcementmaterial): ρc= ρrvr+ρmvm The above expression can be generalized and its general form is known as law of mixture and is given below Xc = XmVm+ XpVpExperimentally, the density of a composite is obtained by displacement techniques  using a physical balancewith density measuring kit as per ASTM: D 792-66 test method. Further, the density can also be calculated fromporosity and apparent density values (sample mass and dimensions) .The results of the several investigations[23-24] regarding the density of the Al2O3 SiC C particle reinforced Al and other aluminum alloys can besummarized as follows: the reinforcements Al2O3SiCC enhance the density of the base alloy when they are added tothe base alloy to form the composite. Moreover, the theoretical density values match with the measured densityvalues of these composites. Further the density of Al203-SiCC particle composites is greater than that of Al203-SiC Cwhisker reinforced composites for the same amount of volume fraction. From the above the increase in density canbe reasoned to the fact that the ceramic particles possess higher density.Further, the increased volume fraction of these particles contribute in increasing the density of the composites, alsothey have stated that the theoretical and measured density values of these composites match to each other.Additionally, the above discussions can be reasoned to the fact that the ceramic particles possess higher density.The reinforcement of aluminium alloys with ceramic particle leads to new generation of engineering materials withimproved mechanical properties to weight ratio [1-3]. Aluminium alloys are still the subjects of intense studies, astheir low density gives additional advantages in several applications. These alloys have started to replace cast ironand bronze, to manufacture wear resistance parts . Previous studies have shown that mechanical properties of Al-matrix composites would be enhanced with particle reinforcement [5-7]. Development of composite materials canbring combined advantages of the constituent materials [8-10]. MMC`s reinforced with particles tend to offerenhancement of properties processed by conventional routes [11, 12]. Al2O3 SiC C is particulate used asreinforcement in Aluminium alloy composites in the present work. But SiC is the most commonly used particleused as reinforcement in Aluminum alloy composites[10, 11]. By adding ceramic particles as reinforcement toAluminium matrix, the properties are enhanced and lead to the development of materials for many lightweightapplications . For production of aluminium particulate reinforced composites stir casting method appears to bepromising method among various conventional processing methods . Heat treatment process to modify themicrostructure of aluminium alloy composites with aluminum alloy matrix is the final production stage ofcomposites [17, 18]. Most of the researchers have investigated aluminium composites using SiC, Al2O3, MgO,Zircon etc, and these composites are commercially available in different structural forms.In this light an attempt has been made to develop Aluminum particulate alloy composites. An effort has been madein this paper to study the particulate and whisker distribution properties of Aluminum alloy composite by varyingthe wt% of the particulate.
Innovative Systems Design and Engineering www.iiste.orgISSN 2222-1727 (Paper) ISSN 2222-2871 (Online)MATERIALS AND METHODSMaterials preparation The Aluminum matrix particulate composite material is manufacturing by the mixing equation as where φ is function and a,b,c,d,e,f,g and h are the constants of the differential function.Pure Al is the matrix material and Al2O3 SiC C is used as reinforcement material in the preparation of composites.The properties of matrix material is shown in Tables 2 and Table 3.A stir casting setup was used consisting of resistance furnace with a mechanical stirrer unit. Approximately 190grams of pure Al ingots were cut in to pieces to accommodate into the graphite crucible. The temperature of thefurnace was raised slowly above liquideous temperature of the melt and then slowly reduced below the liquideoustemperature of the matrix material. Preheating of the particles at 4500 C was done in a muffle furnace, placed nearthe casting set up, in order to remove the moisture and gases from the surface of the particles . The stirrer wasraised, positioned and then lowered into crucible. The speed range was 300-350 rpm. The preheated particles inweighed quantities were added slowly into the melt. After adding the particles, stirring was continued for 10 minutesfor better wetting dispersion. The pouring temperature was maintained at 7100C. Then melt was poured into apreheated metal molds (dies) as shown in Figure 1and Figure 2.RESULTS AND DISCUSSIONSMicrograph studies: The specimen thus cast was studied under an image analyzer. It is very clearly seen that anuniform distribution of flakes was happened to the specimen. The aspect ratio and the quantity of flakes werestudied and tabulated as shown in the table 4, Table 5, Table 6 and Table 7.CONCLUSIONS Based on the experimental observations made in the present research, the following conclusions have been drawn. Al - Al2O3 SiC C particulate composites have been successfully developed with fairly uniform dispersion of the particulate whisker particles. The whisker distribution of particulates of Al - Al2O3 SiC C composite material increases as the addition of Al2O3 SiC C particles weight percentage is increased. This is due to hard Al2O3 SiC C particles dispersion in soft aluminium alloy matrix. Addition of Al2O3 SiC C particles significantly improves ultimate tensile strength of Al6061, when compared with that of unreinforced matrix, the ultimate tensile strength of Al2O3 SiC C composite is increased by 36.71%.
Innovative Systems Design and Engineering www.iiste.orgISSN 2222-1727 (Paper) ISSN 2222-2871 (Online)REFERENCES K.S.Raghuram, Dr.N.V.S.Raju, S.N.Padhi Jan 2010. Strength Properties of in-situ Aluminum Matrix ParticulateComposites by Rheocasting In the proceedings of International Conference on MEMS and OptoelectronicsTechnologies ICMOT – 2010 by IACQER vide page 460 – 463 D.M. Aylor. 1982. Metals Hand Book V-13 & Vol. 19. ASM Metals Park, OH. pp. 859-863. J.P. Pathak, J.K. Singh and S. Mohan. 2006. Synthesis and characterization of Aluminium-Silicon-Siliconcarbide composite. Indian Journal of Engineering & Material Sciences.Vol. 13, June. pp. 238-246.  Hashim J.,LooneylHashmi M.S.J. 1999. J. Master. Process Technol. 92-93: 1. Sanchez-Santana, U. Rubio-Gonzalez, C. Gomez-Rosas, G. Ocan, J.L. Molpeceres, C. Morales. 2006. Friction of6061-T6-aluminium alloy treated by laser shock processing. Wear. 260: 847-854. Qianz Zhang, Gaohai Wu, Longtao Jiang. 2008. Tensile deformation behavior of a sub-micrometer Al2O3/ 6061Al composite.Material Science and Engineering. pp. 483-484, 281-284.  RupaDasgupta, HumairaMeenai. 2003. SiC particulate dispersed composites of an Al-Zn-Mg-Cu alloy; propertycomparison with parent alloy. Materials characterization. 54: 438-455. Pitcher P.D, Shakesheft A.J, Lord J.D. 1998. Aluminium based metal matrix composites forimproved elevated temperature performance. Mater. Sci. Technol. 14: 1015-1023. Shakesheff A.T, Purdie G. 1998. Designing metal matrix composites to meet their target: Particulate reinforcedAl alloys for missile applications. Material Science Technol. 14: 851-856. A.K. Banerjee, P.K. Rohatgi, W. Reif. 1985. In: Proceedings of the eight symposiums in Advanced MaterialsResearch and Development for TansportComposites.Stravsbourg, France.November. H.B. Niranjan. 1998. Tensile and Corrosive properties of Al Haematite composite. In: Proceedings of the firstAustralasian Conference on Composite Materials (ACCM –I), Osaka Japan. 7-9 October.p. 546. J. Gurlond. 1974. Composite Materials. In: L.J. Brautman (Ed.). Vol. IV. Academic Press, New York. K.S.Raghuram, Dr. N.V.S.Raju.2010 Manufacturing results of aluminum matrix composite materials reinforcedby in-situ Al2O3 SiC C particles special issue of Bionano Frontier, a journal of International Society of Science &Technology, Mumbai.
Innovative Systems Design and Engineering www.iiste.orgISSN 2222-1727 (Paper) ISSN 2222-2871 (Online) Table 2 showing thedensities of matrix and Table 3 showing the %wt composition of matrix materialparticulate material in Spot Al Si Ca S Ti Fe Cu gm/cm3 1. 90.837 7.629 0.204 0.00 0.341 0.341 0.995 Pure Al 2.7 Al2O3 3.89 SiC 3.21 C 1.98Figure 1and Figure 2. showing the particulate distribution in the Al- Al2O3 SiC C composite material under ImageAnalyzer.Table 4 showing the frames, area of frames and number of flakes
Innovative Systems Design and Engineering www.iiste.orgISSN 2222-1727 (Paper) ISSN 2222-2871 (Online)Table 5, Table 6 and Table 7